The α ↔ β phase transitions of Zn2P2O7 revisited: existence of an additional intermediate phase with an incommensurately modulated structure.
Stöger, Berthold; Weil, Matthias; Dušek, Michal; Acta Crystallographica, Section B: Structural Science, Crystal Engineering and Materials 70 (2014) 539–554; doi:10.1107/S205252061401049X

data_2310795
_publ_section_title
;
 The \a &#x2194; \b phase transitions of Zn2P2O7 revisited: existence of
 an additional intermediate phase with an incommensurately modulated
 structure.
;
_journal_coden_ASTM              ACSBDA
_journal_issue                   3
_journal_name_full
;
 Acta Crystallographica, Section B: Structural Science, Crystal Engineering
 and Materials
;
_journal_page_first              539
_journal_page_last               554
_journal_paper_doi               10.1107/S205252061401049X
_journal_volume                  70
_journal_year                    2014
_chemical_formula_sum            'O7 P2 Zn2'
_chemical_formula_weight         304.7
_chemical_name_common            'zinc pyrophosphate'
_chemical_name_systematic        'zinc(II) diphosphate(V)'
_space_group_IT_number           12
_space_group_ssg_name            C2/m(\a0\g)0s
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.335(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.5998(4)
_cell_length_b                   8.2845(5)
_cell_length_c                   4.5300(3)
_cell_measurement_reflns_used    3836
_cell_measurement_temperature    500
_cell_measurement_theta_max      45.3
_cell_measurement_theta_min      4.0
_cell_modulation_dimension       1
_cell_volume                     238.86(3)
_computing_cell_refinement       'SAINT-Plus (Bruker, 2012)'
_computing_data_collection       'APEX2 (Bruker, 2012)'
_computing_data_reduction        'SAINT-Plus (Bruker, 2012)'
_computing_molecular_graphics    'ATOMS (Dowty, 2006)'
_computing_structure_refinement  'JANA2006 (Pet\<r\'i\<cek, et al., 2006)'
_computing_structure_solution    'by isomorphous structure methods'
_diffrn_ambient_temperature      500
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 1
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Bruker KAPPA APEX II CCD'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0248
_diffrn_reflns_av_unetI/netI     0.0296
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_index_m_1_max 1
_diffrn_reflns_limit_index_m_1_min -1
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            8052
_diffrn_reflns_theta_full        45.37
_diffrn_reflns_theta_max         45.37
_diffrn_reflns_theta_min         3.47
_exptl_absorpt_coefficient_mu    10.69
_exptl_absorpt_correction_T_max  0.60
_exptl_absorpt_correction_T_min  0.025
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            'translucent colourless'
_exptl_crystal_density_diffrn    4.2351
_exptl_crystal_description       rod
_exptl_crystal_F_000             292
_exptl_crystal_size_max          0.42
_exptl_crystal_size_mid          0.30
_exptl_crystal_size_min          0.06
_refine_diff_density_max         1.04
_refine_diff_density_min         -1.13
_refine_ls_extinction_coef       2750(110)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    2.18
_refine_ls_goodness_of_fit_ref   1.50
_refine_ls_number_constraints    1
_refine_ls_number_parameters     98
_refine_ls_number_reflns         2969
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0653
_refine_ls_R_factor_gt           0.0295
_refine_ls_shift/su_max          0.0199
_refine_ls_shift/su_mean         0.0034
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0445
_refine_ls_wR_factor_ref         0.0467
_reflns_number_gt                1331
_reflns_number_total             2969
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            xk5017sup1.cif
_cod_data_source_block           alpha2_zn2p2o7_500
_cod_database_code               2310795
_publcif_datablock.id            {03a808b6-1ffd-41e5-9f37-11d932d00315}
_publcif_info_exptl_table_max_cols 5
_publcif_info_exptl_table_use_headnotes n